HAL Id: hal-02408292
https://hal.archives-ouvertes.fr/hal-02408292Submitted on 16 Dec 2019
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Probing the thermal effects of voltage hysteresis in
anionic redox-based lithium-rich cathodes using
Gaurav Assat, Stephen Glazier, Charles Delacourt, Jean-marie Tarascon
To cite this version:
Gaurav Assat, Stephen Glazier, Charles Delacourt, Jean-marie Tarascon. Probing the thermal ef-fects of voltage hysteresis in anionic redox-based lithium-rich cathodes using isothermal calorimetry. Nature Energy, Nature Publishing Group, 2019, 4 (8), pp.647-656. �10.1038/s41560-019-0410-6�. �hal-02408292�
- 1 -
Probing the thermal effects of voltage hysteresis in
anionic-redox-based lithium-rich cathodes using isothermal calorimetry
Gaurav Assat,1,2,3 Stephen L. Glazier,4 Charles Delacourt,*,2,5 Jean-Marie Tarascon*,1,2,3
1 Collège de France, Chimie du Solide et de l'Energie - UMR 8260 CNRS, 11 Place Marcelin Berthelot, 75005
2 Réseau sur le Stockage Electrochimique de l’Energie (RS2E) - FR CNRS 3459, 80039 Amiens Cedex, France 3 Sorbonne Université – UPMC Paris 06, 4 Place Jussieu, 75005 Paris, France
4 Department of Physics and Atmospheric Science, Dalhousie University, Halifax, N. S., B3H 4R2, Canada 5 Laboratoire de Réactivité et Chimie des Solides (LRCS) - UMR CNRS 7314, Université de Picardie Jules
Verne, 33 rue Saint Leu, 80039 Amiens Cedex, France
* Corresponding authors:
C. Delacourt: email@example.com
- 2 -
The commercialization of high-energy batteries with Li-rich cathode materials exhibiting
combined cationic/anionic redox processes awaits the elimination of certain practical bottlenecks.
Among these, large voltage hysteresis remains the most obscure from a fundamental
thermochemical perspective. Here we study this issue by directly measuring via isothermal
calorimetry the heat generated by Li/Li2Ru0.75Sn0.25O3 (Li/LRSO) cells during various cycling 5
conditions, with LRSO being a ‘model’ Li-rich layered cathode. We show how this heat
thermodynamically relates to the lost electrical work that is crucial for practical applications. We
further reveal that anionic redox on charging and discharging adopts different metastable paths
having non-identical enthalpy potentials such that the overall Li content no longer remains the
unique reaction coordinate, unlike in fully path-reversible cationic redox. We elucidate how
static voltage hysteresis is related with heat dissipated due to non-equilibrium entropy production.
Overall, this study establishes the great benefits of isothermal calorimetry for enabling energy
efficient electrode materials in next-generation batteries.
- 3 -
Increasing the energy density of lithium-ion batteries requires denser positive electrodes
with higher voltage and/or capacity. Li2MnO3-based Li-rich layered oxides (Li-rich NMCs), such as 15
Li1.2Ni0.13Mn0.54Co0.13O2, can deliver specific capacities above 270 mAh g–1 to reach 1000 Wh kg–1 16
of specific energy at the material level. Despite their slightly lower crystalline density than today’s
Li-stoichiometric Ni-based layered oxides (NMCs and NCA), Li-rich cathodes remain very
promising for the long-term, as we will need to move away from Ni-rich towards Mn-rich materials
(Mn is inexpensive and environmentally benign) without compromising the energy density.1–3 The
high capacity of Li-rich NMCs stems from cumulative anionic and cationic bulk redox processes.4–
6. However, these electrodes currently fall short in other performance metrics7 because of large 22
voltage hysteresis5,8, sluggish kinetics5,9,10, and gradual voltage fade11. These issues are concomitant
with anionic redox activity7 – the very same feature that enhances capacity. Therefore, further
investigations are needed to fundamentally understand the overall anionic redox process, which
constitutes not just of electron removal from oxygen-based electronic states, but also the ensuing
(local) structural/bonding rearrangements.7 27
The undesirable issue of voltage hysteresis in rechargeable batteries leads to energy
inefficiency, presumably dissipated as heat, consequently imposing an additional energy cost on the
end-users.12 Voltage hysteresis would also complicate the state of charge (SoC) and thermal
management of such batteries. Li-rich NMCs show a relatively large difference between
charge/discharge voltages (~400–500 mV after first cycle, ~87% energy efficiency, Figure 1). This
gap persists over cycling, even at extremely low rates (C/300)10, at high temperatures (55 or 85
°C)13, and after long relaxation periods (100 hours)10. Such behaviour therefore cannot be explained
by simple electrochemical kinetics that fails to explain the observed path dependence and
static hysteresis. Interestingly and similar to Li-rich NMCs, many other newly-discovered Li- and
Na-based materials with reversible anionic redox also suffer from voltage hysteresis.7 These include
- 4 -
layered Li2Ru1–xSnxO39 (Figure 1), Na2/3[Mn1–xMgx]O214, and Na2RuO315 as well as disordered 38
Li1.2Mn0.4Ti0.4O216 and Li2MnO2F17. 39
Only a few studies have attempted to understand the origin of voltage hysteresis in this class
of cathodes. These include electrochemical measurements in different voltage windows to identify
correlated differential capacity ( ⁄ ) peaks5,8,11,18,19, 6Li nuclear magnetic resonance to observe
path-dependence in lithium site occupation20, X-ray diffraction to claim back-and-forth (partially
reversible) transition-metal migration21, and bulk X-ray spectroscopies5,22,23 to demonstrate the
absence of hysteresis in the potentials at which transition-metals show redox-activity, unlike for the
hysteretic oxygen redox process. A couple of phenomenological models assuming either a Li-driven
phase change10 or an asymmetry in transition-metal migration24 were also conceived. Despite such
widespread efforts, the general thermodynamic mechanism behind voltage hysteresis and its
thermal effects remain unclear. Two questions need answering: (i) how exactly is the lost energy
dissipated as heat so that it can be better managed/predicted? and (ii) what is the underlying
mechanism along with the corresponding thermochemical conditions that lead to hysteresis?
In light of this, we adopt a different approach herein and perform isothermal calorimetry
measurements during the cycling of a ‘model’ Li-rich layered cathode – Li2Ru0.75Sn0.25O3 (LRSO) 53
or Li[Li0.33Ru0.5Sn0.17]O2. This high capacity (~250 mAh g–1 reversibly) material, although only 54
suitable for niche applications without cost batteries (e.g. space), shows remarkable structural and
electrochemical similarities with the practically important Li-rich NMCs (Figure 1).9,25 . Overall, it
serves as a simplified ‘model’ compound to understand the general properties of Li-rich layered
electrodes. The magnitude of voltage hysteresis in LRSO (~200–300 mV) is lower than Li-rich
NMCs but the role of anionic redox activity is particularly similar, such that high potential charging
triggers the onset of hysteresis.9,23 Using isothermal calorimetry in this work, we report the heat
generation during different electrochemical stages of LRSO, starting with the classical cationic
redox step in first charge followed by the voltage plateau accompanying oxygen redox and finally
- 5 -
the hysteretic sloped voltage profiles that stabilize over cycling. These measurements allow us to
discuss the thermodynamics in terms of enthalpy change, entropy change, and entropy production.
We highlight the thermal asymmetry in the charge vs. discharge paths as well as the difficulties in
locating the true equilibrium properties of such hysteretic materials. A multi-step reaction scheme
for the solid-state oxygen redox reaction is finally proposed to comprehend the results.
Figure 1 | Comparison of voltage profiles of Li-rich NMC and LRSO. The first cycle (a and b)
displays a two-stepped charge followed by a sloped discharge. The labels “C” and “A” denote respectively the cationic and anionic redox processes. The later cycles (c and d) display a quasi-static voltage hysteresis, leading to an energy inefficiency that is equivalent to the shaded area between the charge and discharge profiles. In a and b, the materials do not get back to their initial states after the first cycle, unlike for the already-formed materials in c and d.
The heat generated by an electrochemical cell in isothermal and isobaric conditions is
described in the Methods section.26,27 Because of large voltage hysteresis and path-dependence in
Li-rich cathodes5,9, the position of their equilibrium potential cannot simply be assumed in the 70
middle of the charge and discharge, unlike in classical path-reversible intercalation materials. We
therefore need a different approach herein. Neglecting heat of mixing27,28 and correcting for minor
parasitic heat flow (see details in Methods), the energy balance can be recast as
− | , = − =
- 6 - with 75 = −∆ Equation  76 77
where is the cell voltage, | , is the heat generation rate (positive if heat is released by
cell), is the current (positive for charging), is the temperature, is the surrounding pressure,
is the number of electrons involved in electrode reaction, is the Faraday’s constant, and is the
so-called “enthalpy potential”.27 Just as is directly related to the partial change in Gibbs free
energy of the cell as its SoC is varied ( = −∆ ), is directly related to the partial change in the
enthalpy of the cell. In other words, captures the energy change while includes the entropy
change as well. can thus simply be obtained by measuring , , and | , . Knowing can help
in predicting the heat generation under operating conditions for proper thermal management of
Equation  over a closed path, such as a charge–discharge cycle after which the material
returns to its original state, gives
89 = | , Equation  90 91
because enthalpy is a state variable and cancels out over a stable cycle as follows
92 93 = − = 0 Equation  94
- 7 -
Equation  demonstrates that the net electrical work due to hysteretic voltage profiles is
dissipated as waste heat. Note that the measured via
Equation  (under applied current) can be path dependent, i.e. different on charge vs.
discharge for the same SoC, if the materials inside the cell remain as metastable phases under
dynamic conditions away from the true equilibrium. Nevertheless, even in that non-equilibrium
case, over a stable cycle (i.e. having no net change in ) is constrained by Equation  and
therefore cannot form a hysteretic loop versus Li composition , as schematized in Supp. Figure 1.
Note that Li-rich materials do not have a perfectly stable cycle because of gradual voltage fade.
However, these changes will turn out to be negligible for LRSO later in the paper.
In addition to the above energy balance, the Second Law of Thermodynamics relates the
entropy change to the heat exchange as29 106 | , = − + , ≥ 0 Equation  107 108
where is the rate of entropy change of the cell and is the rate of entropy production
due to the irreversible processes inside the cell. is close to zero only over a
thermodynamically reversible path. Since entropy is a state variable, its integration over a closed
path (e.g. a stable charge–discharge cycle) becomes
112 113 = = 0 Equation  114 115
- 8 -
Consequently, the integration of Equation  over a closed path, when combined with
116 Equation , gives 117 118 = | , = ≥ 0 Equation  119 120
The overall voltage hysteresis (both resistive and current-independent in nature) is therefore
a measure of entropy production that is dissipated as heat. Entropy production in the realm of
chemical reactions29 is further described along-with
Supp. Figure 2.
Isothermal calorimetry results for the 3.5 V cationic redox
Initial electrochemical de-intercalation of up to 0.75 Li per formula unit from
Li2Ru0.75Sn0.25O3 (LRSO) takes place around 3.5 V with the oxidation of primarily Ru-based 125
electronic states (hence termed cationic redox). This redox step is completely reversible.9,23
Isothermal calorimetry measurements at 40 °C (see Methods for details) were performed over this
step in coin-type Li half-cells at different C-rates, ranging from C/20 to C/5. Figure 2a shows the
resulting voltage profiles, which were used along with the simultaneously measured heat flow rates
to obtain the profiles of enthalpy potential using
Equation , as shown in Figure 2b for the slowest rate of C/20. The symmetric shape of
the heat flow profiles (orange curves) arises because of reversible entropic heat, whereas the net
positive shift is due to irreversible heat from overpotential (see Methods for further explanations).
The calculated profiles (pink curves) superimpose neatly on charge and discharge, indicating
that the enthalpy change is path independent (Supp. Figure 1a) and is only a function of the Li
- 9 -
stoichiometry (SoC). Such behaviour is typical for classical electrochemical intercalation
reactions.26,30 Understanding the exact shape of entropic heat flow is beyond the scope of this study,
as it may be related to many aspects of the cathode material, such as the changes in Ru–Ru bond
distance ordering23, charge ordering, Li vacancy ordering, or the shape of the ⁄ profile (Supp.
The deviation (early drop, marked by green arrows) of the discharge profile from that on
charge in Figure 2b is likely because of concentration gradients and can be understood better by
studying the effect of varying C-rates. The profiles obtained at different rates are compared in
Figure 2c (see Supp. Figure 4 for the raw heat flow profiles). They converge over a broad range of
SoCs for both charge and discharge, however with some rate-dependent discrepancies at the
extremities, as highlighted with green backgrounds in Figure 2c. These kinetic effects arise from
the formation and relaxation of concentration gradients, most likely in the solid phase due to limited
lithium diffusion since the electrode is designed with a high (~60 %) porosity (electrode details in
Methods), and the associated heat of mixing effects27,28 that were neglected in
Equation . Nevertheless, the profiles at the slowest rate superimpose adequately and
reflect the enthalpy change of the electrochemical reaction. Moreover, the voltage and heat profiles
remain perfectly identical over consecutive cycles in this cationic redox regime (Supp. Figure 5).
Lastly, Figure 2d compares the net electrical work and the net heat generated from the cell
over a complete cycle at different rates. The heat and work are positive and match with each other,
in agreement with Equation . Moreover, they exhibit a linear relationship with current that
approaches close to zero as the current diminishes. Overall, the calorimetric analysis of the 3.5 V
cationic redox step demonstrates its classical nature, i.e. it is path independent with minor
static voltage hysteresis, and can be thermodynamically treated as a single-step electrochemical
- 10 -
Figure 2 | Isothermal calorimetry characterization of the 3.5 V cationic redox step. Voltage
profiles (a) obtained with LRSO cycled inside the calorimeter at 40 °C using CCCV protocols after a few formation cycles. The polarization gradually increases with increasing C-rates. For C/20 (b), the measured profiles of cell voltage (blue) and heat flow rate (orange) that were used to obtain the
profiles (pink). lies above the equilibrium potential located somewhere between the
charge and discharge voltages. Therefore, the entropic term is such that the cell’s entropy increases on charge (causing heat absorption) and decreases on discharge (causing heat release). (c)
Convergence of profiles obtained at different rates, with green backgrounds highlighting the
deviations possibly due to heat of mixing.As the C-rate increases, the charge profiles develop a
small distortion at the onset of charge and show an early rise towards the end of charge. Similarly,
the discharge profiles show an early drop towards the end of discharge. (d) Comparison of lost
electrical work with dissipated waste heat over complete charge–discharge cycles.The slope and
intercept are respectively related to the “SoC averaged” values of and in Equation
Error! Reference source not found..
Isothermal calorimetry results for the 4.2 V anionic redox
Further extraction of Li from LRSO takes place at the 4.2 V plateau (Figure 3a), which is
charge-compensated by the oxidation of bulk lattice oxygen (electron removal from oxygen
bonding levels, hence termed anionic redox).7,23 This step releases significantly larger heat than the 162
preceding cationic redox (Figure 3b). Such a large heat release cannot simply be explained by
electrochemical resistance, which we previously showed to remain small.9 We had additionally
reported very slow equilibration dynamics, such that the open-circuit voltage (OCV) slowly relaxes
away from the voltage under load for long periods of time. Note in this case that the direct
determination of the entropic term by temperature-dependent potential measurements, as
attempted for Li-rich NMC31, is questionable. Structure-wise, the anionic redox plateau leads to a 168
loss of crystallinity along with the onset of local distortion, in contrast to the preceding cationic
step.23,25 Moreover, the subsequent discharge adopts a different sloped S-shaped path (
All these observations indicate that the 4.2 V plateau is an electrochemically-driven irreversible
- 11 -
phase transformation (hereafter termed as ‘activation’) from the crystalline partially-charged phase
to the disordered/distorted fully-charged one. This is reminiscent of conversion-type electrode
materials and cannot be treated as a single-step electrochemical reaction. We therefore propose a
two-step electrochemical/chemical (EC) mechanism to explain the anomalous heat generation. The
electrochemical (E) step consists of electron removal from states derived primarily from oxygen
(anionic oxidation) and the follow-up chemical (C) step is a stabilizing structural rearrangement,
e.g. the distortion of RuO6 octahedra leading to the shortening of O–O distances and/or metal-ion 178
migration.7,23,25 This stabilizing chemical step explains the large heat generation observed over the
The profiles obtained from
Equation  are shown in Figure 3c. Note that these represent the overall changes in the
cell’s enthalpy (without any distinction of the underlying steps). Since the profile on discharge
is well separated from the one on charge, as indicated by a double-headed arrow in Figure 3c, the
condition in Equation  cannot be fulfilled over the first cycle. Hence, there is a net change in
enthalpy, as further schematized in Supp. Figure 1b. In other words, the material does not return to
the pristine state after a full charge–discharge cycle, consistent with previous
characterizations.23,25,32 In summary, the large heat release during the voltage plateau may be due to 188
the underlying rearrangement step that accompanies anionic oxidation. The subsequent discharge
follows a thermodynamically different path.
Figure 3 | Isothermal calorimetry characterization of the full first cycle. (a) Voltage profile
(blue) and (b) heat flow profile (orange) for the staircase-like first charge, followed by an S-shaped sloped discharge. An unintended interrupt of 104.4 mins (marked by *) occurred during the anionic oxidation plateau, which is further described in Supp. Figure 6. The steep rise in heat release at the end of the plateau is unrelated to the current interrupt and may be explained by the expected rise in
- 12 -
irreversible heat contribution due to poor kinetics when the reaction approaches its end. Other
possibilities include partial oxygen release25 and/or side reactions, possibly correlated with the
small voltage feature near 4.5 V. The cell used here was the same as the one in Figure 2 on partial cycling (cationic redox only), which is overlaid here for comparison with the full cycle. (c) The calculated enthalpy potential profiles (pink) are shown along with the cell voltage profile over the complete first cycle. A double-headed green arrow highlights the separation between charge versus discharge enthalpy potentials.
Isothermal calorimetry results for ‘activated’ LRSO
After some formation cycles, LRSO’s sloped S-shaped voltage profiles stabilize, with nearly
equal capacity contributions from cationic and anionic redox processes that take place at low and
high potentials respectively.9,23 To understand the electrochemical mechanism of this ‘activated’
phase, isothermal calorimetry was performed at different rates ranging from C/50 to C/5. The
resulting voltage profiles exhibit a significant voltage hysteresis that does not diminish by lowering
the current (Figure 4a). The heat flow for the slowest rate of C/50 (Figure 4b) is not symmetric
and remains largely above zero for the entire cycle, unlike the classical cationic redox in previous
Again, the profiles were calculated from
Equation , as shown in Figure 4b for C/50 (other rates in Supp. Figure 8, comparison
with initial cycle in Supp. Figure 9). Interestingly, the profiles on charge vs. discharge are
much closer in comparison to the hysteretic voltage profiles. A larger heat generation on discharge
indicates that the reaction’s enthalpy potential is located further away from the discharge voltage
than the charge voltage. Note that, despite a low rate of C/50, the profiles on charge and
discharge do not fully superimpose, especially in the second half of SoCs (anionic redox region),
thus reflecting a slight path dependence in the cell’s enthalpy, as also schematized in Supp. Figure
1c. This effect was consistently observed for several cells (Supp. Figure 10). Whether this slight
mismatch is due to kinetic or thermodynamic reasons can be understood from Figure 4c. On either
- 13 -
charge or discharge, the profiles obtained at different rates converge over almost the entire SoC
range, except possible heat of mixing effects at the end of charge and the beginning of discharge
(highlighted with green backgrounds). Therefore, enthalpy-wise, the charge and discharge paths are
rate-independent over the range of rates studied herein (from C/50 to C/5). Moreover, these paths
are slightly dissimilar as they do not converge to a single unique curve. ‘Activated’ LRSO thus
follows metastable paths having slightly different enthalpies on charge vs. discharge for the same
SoC. Therefore, the overall Li content is no longer the unique reaction coordinate to fully describe
the system, as discussed later.
Nevertheless, since ‘activated’ LRSO shows fairly stable heat profiles with negligible
voltage fade in consecutive cycles (Supp. Figure 11), the profiles should satisfy Equation ,
despite being slightly different on charge vs. discharge, as also schematized in Supp. Figure 1c.
This can be verified from Figure 4d showing the match between net heat and work (over complete
cycles). The extra work needed due to voltage hysteresis is therefore dissipated as heat. The
current intercept in Figure 4d is large (~70.4 Wh kg–1), unlike Figure 2d, because of the large
quasi-static hysteresis. It is key here to note that this significant dissipation can be viewed,
according to Equation , as entropy production and implies that the underlying steps are far away
from equilibrium even at the lowest rates (further discussion with Supp. Figure 2). Entropy
production (the value of the integrals in Figure 4d) should ideally vanish to zero at infinitesimally
small rates at which all the underlying steps would be near equilibrium. However, demonstrating
this is not trivial simply due to prohibitively long experiments as well as the interfering
reactions at extremely low C-rates. Such non-equilibrium arguments also explain the continuous
voltage relaxation observed for LRSO under open circuit conditions, despite long time periods (24
hours)9, because some of the underlying steps have slow equilibration dynamics with very large
time constants. Since similar slow dynamics plague Li-rich NMC10, equilibrium is never achieved
and the reported values of the entropic term are invalid as they violate Equation  during the
- 14 -
sloped cycles31. Likewise, distinguishing the true equilibrium potential (unique) from
dependent metastable equilibrium potentials (non-unique) requires further thermodynamics
Overall, it is clear that voltage hysteresis is linked to non-equilibrium entropy production,
which can be quantified over a complete cycle as the net dissipated heat or lost electrical work.
However, further deconvolution of the heat flow rate into entropy change and entropy production
rates, as per Equation , is not possible without precise knowledge of the underlying mechanism.
Therefore, a multi-step mechanism consistent with calorimetry results is presented later.
Figure 4 | Isothermal calorimetry characterization of ‘activated’ LRSO. The hysteretic voltage
profiles (a) obtained with LRSO cycled inside the calorimeter using CCCV protocols. ⁄
curves are shown in Supp. Figure 7. The experiments were performed after a few formation cycles
in the full potential range leading to complete ‘activation’.The quasi-static hysteresis appears to be
larger in the higher potential anionic redox range. For C/50 (b), the measured profiles of cell
voltage (blue) and heat flow rate (orange) that were used to obtain the profiles (pink). A zoom
in inset shows the slight differences in profiles over the high potential region. (c) Convergence
of profiles obtained at different rates for charge (top) and on discharge (bottom), with green
backgrounds highlighting the deviations possibly due to heat of mixing. (d) As a function of C-rate, the comparison of lost electrical work with dissipated waste heat over a complete charge–discharge cycle obtained by integrating respectively the cell voltage and the heat flow rate. These integrals scale linearly with current, with the slope and intercept respectively related to the “SoC averaged”
values of and in Equation Error! Reference source not found..
Voltage window opening experiments were next performed. Figure 5a reveals that charging
to high potentials, particularly beyond 50% SoC, gradually triggers voltage hysteresis. Akin to the
discharge voltage profiles that are path dependent (i.e. they depend on the extent of charging), the
discharge heat flow profiles (Figure 5b) also exhibit path dependence. Consistent with voltage
hysteresis, discharging from the fully charged state results in a larger heat generation over a broad
range of SoCs (denoted by arrows) compared to discharge from partially charged states. The
- 15 -
corresponding discharge profiles (Figure 5c) in the lower half of SoCs (cationic redox23)
converge independently of the charging history. In contrast, for the upper half of SoCs (anionic
redox23), the discharge curves gradually evolve as a function of the extent of charge, thus
highlighting the distinctive role of the anionic redox process in causing voltage hysteresis. Lastly,
the net heat and work over complete cycles are compared in Figure 5d as a function of the charging
SoC. They again match with each other, consistent with Equation . Instead of a linear trend with
current that is expected for path reversible intercalation materials, a non-linear rise is observed in
Figure 5d because of gradually worsening voltage hysteresis as the charging voltage window is
opened. In light of these unusual observations triggered by high potential charging, a multi-step
mechanism for the anionic redox process is proposed next.
Figure 5 | Isothermal calorimetry for charge voltage window opening of ‘activated’ LRSO. (a)
Voltages profiles (blue). ⁄ curves are shown in Supp. Figure 12. (b) Heat flow profiles
(orange) on discharge only. Complete heat profiles in Supp. Figure 13. (c) The calculated
profiles (pink, for discharge only). profiles on charge are identical as expected (see Supp.
Figure 14). A dashed curve in the background shows the full range charge–discharge voltage
profile. The initial kinks in profiles at the onset of discharges is likely due to heat of mixing, as
also observed in Figure 4c. (d) As a function of SoC to which the cell is charged, a comparison of lost electrical work with dissipated waste heat over a complete charge–discharge cycle obtained by
integrating respectively the cell voltage and the heat flow rate. This non-linear trend was verified
with a second cell (Supp. Figure 15).
Proposed multi-step mechanism for hysteretic anionic redox
The mechanism behind the hysteretic anionic redox process in ‘activated’ LRSO can now
qualitatively be understood in light of the above calorimetry results. From the point of view of local
structure, cationic redox can be treated as a single electrochemical step, therefore free from
static voltage hysteresis (Figure 6a). On the other hand, anionic redox can be described as a
- 16 -
step process, consisting of sequential redox (electrochemical) and rearrangement (chemical) steps,
which form a “square-scheme”33–35 (Figure 6b) having a reaction energy landscape shown in
Figure 6c. On charge, the electrochemical oxidation of anions is followed by a stabilizing structural
rearrangement that could either enlist the distortion of octahedral symmetry leading to O‒O
shortening7,23, metal-ion migration6,8,11,20,21, or a layer stacking change14,15. Owing to this structural 266
modification, a different redox step is needed on discharge, which is again followed by a stabilizing
rearrangement to the original state with reduced anions. Interestingly, these steps are analogous to
the “square-scheme” mechanism that causes voltage hysteresis in certain molecular machines.34–36
Note that the four elementary steps are thermodynamically constrained as they form a closed cycle,
but they do not necessarily take place close to equilibrium. A complementary experiment of
gradually opening the discharge voltage window (Supp. Figure 16) fully supports the proposed
Such a multi-step mechanism allows for non-equilibrium to exist if the kinetics of some of
the elementary steps, most likely the chemical rearrangements steps, is slow enough (much slower
than the C-rates used). In such a non-equilibrium case, the overall Li content of the electrode
material is not the only reaction coordinate (the other coordinates being related to species
repartitioning). The persistence of metastable paths can thus be explained, such that, independent of
current, charge predominantly occurs via the upper path in Figure 6b and discharge via the lower
one. Therefore, the non-equilibrium cell potentials during charge and discharge are respectively
closer to the thermodynamic potentials and of the two redox steps, hence giving rise to
voltage hysteresis. This hysteresis leads, by definition, to dissipative entropy production29, whose
value on charge and discharge is in part related to the Gibbs free energy of reaction of the respective
rearrangement step (Figure 6c). Nevertheless, the exact mathematical form of entropy production,
as described along-with Supp. Figure 2, depends on the underlying thermodynamics and kinetics
of the elementary steps that are, unfortunately, not easy to parametrize for LRSO. Thus, novel
- 17 -
methods need to be developed for determining the entropy change for such path-dependent
materials that show continuous OCV drift. Note that true equilibrium theoretically does exist in the
scheme of Figure 6b, i.e. when the four steps occur in unison, but this situation is never achieved at
practical C-rates,hence leading to metastability. This is the key difference in comparison to cationic
redox, which also involves local structural changes (RuO6 octahedral expansion/contraction and 291
Ru–Ru distance change). However, these changes are energetically small and/or kinetically fast,
and therefore always in equilibrium with the redox step.
Concerning practical applications, the obstacle of quasi-static voltage hysteresis in Li-rich
electrodes can only be overcome by addressing directly the anionic redox process that triggers
atomic motion that is either kinetically slow and/or thermodynamically large in energy penalty,
hence causing metastable reaction pathways and voltage hysteresis. Towards these goals, revisiting
anionic redox chemistry in chalcogenides37, owing to their lower chemical hardness, may prove
beneficial for fundamental understanding of the root cause behind hysteresis. Likewise,
free anionic redox in Na4/7[□1/7Mn6/7]O2 calls for further investigation of Na-based cathodes.38 300
Figure 6 | Proposed mechanism for hysteretic bulk anionic redox in ‘activated’ LRSO. (a)
Cationic redox can be described as a single step electrochemical reaction. C and C+ are the reduced
and oxidized cationic species (e.g. Ru4+ and Ru5+). (b) Anionic redox is described by a multi-step
“square-scheme” mechanism. A denotes the anionic species in reduced state (e.g. O2–) that upon
oxidation forms unstable A+ (e.g. On– with n < 2). Structural reorganization spontaneously takes
place to form stabilized Ar+ (e.g. dimerized O–O2n– with possible metal-ion migration6,7). Reduction
on discharge goes through the unstable Ar (e.g. O–O4–) that spontaneously rearranges back to the
original state. A+ and A
r are therefore the high-energy intermediates for the two respective paths.
Note that electrons and Li ions are not explicitly shown in these schemes. Also, the cationic and anionic reactions may occur in a partially overlapped fashion depending of the precise kinetic and thermodynamic parameters. (c) A schematic reaction energy landscape, highlighting (i) the downhill nature of chemical (C) rearrangement steps, and (ii) their associated kinetic barriers. These two conditions explain path-dependence. If the larger heat generation experimentally observed on discharge is assumed primarily due to entropy production (i.e. minor contributions from reversible
- 18 -
dissociation is energy-wise costlier than its formation.
The above mechanism bears a similarity with the previously proposed “activated bonding
change” model for hysteretic hydrogen-containing carbons39,40, or the phase-change-based model
for hysteretic Li-rich NMC10,24, or the model based on limited ionic mobility for certain hysteretic
displacement reactions41. All these models lead to a non-equilibrium situation under operating
conditions, thus making it necessary to consider the heat associated with bonding change or phase
change, like previously done for hysteretic carbons.42
Lastly, apart from providing mechanistic insights about anionic redox in Li-rich electrodes,
this work provides a new direction in the characterization of batteries with isothermal calorimetry.
A particular highlight is the importance of , the enthalpy potential, that can greatly help in
predicting the total heat generation needed for battery thermal management. Therefore, we
recommend the measurement of , especially for battery materials that either show large entropy
changes or a quasi-static voltage hysteresis (silicon, graphite, LiFePO4, Li-S, Li-O2, and conversion 312
electrodes). The non-equilibrium thermodynamics approach developed herein could be extended to
electrochemical systems beyond batteries, such as water-splitting catalysts showing large
overpotentials or to hysteretic solar cells.
In summary, isothermal calorimetry has elucidated the general thermodynamic mechanism
governing the ‘model’ Li-rich Li2Ru0.75Sn0.25O3 (LRSO) cathode’s electrochemistry. We proved 317
that charging LRSO through the anionic oxidation plateau leads to heat generation and a permanent
change of the material, such that it displays sloped and hysteretic voltage profiles with reversible
oxygen redox chemistry in the subsequent cycles. In a thermodynamically consistent manner, we
demonstrated that the electrical work lost due to such voltage hysteresis is dissipated as waste heat.
It is now clear that (i) metastable paths persist even under quasi-static conditions and that (ii)
- 19 -
voltage hysteresis is directly related to non-equilibrium entropy production instead of simply
originating from large differences in the enthalpy of charge vs. discharge paths.
equilibrium is therefore an essential condition for quasi-static voltage hysteresis, which renders the
estimation of true equilibrium properties quite difficult. The extension of this work to the ‘practical’
Li-rich NMC, among other anionic redox cathodes, is imminent and similar results are expected.
Furthermore, the implementation of model-based simulations could help in generalizing the
step “square-scheme” model proposed herein. Such fundamental understanding is necessary for
designing effective mitigation approaches that can lead to the eventual elimination of voltage
hysteresis. In the broader context, this new direction for battery characterization using isothermal
calorimetry would encourage the electrochemistry community to further exploit this tool as well as
to adopt the concepts of enthalpy potential and non-equilibrium entropy production. From an
applied perspective, the methodology developed herein calls for revisiting some known hysteretic
materials (silicon, conversion-based) and would also help in screening emerging materials for
minimizing heat generation.
- 20 -
Energy balance for an electrochemical cell. The general energy balance for an
electrochemical system was derived by Newman and co-workers.27,43,44 For a thermally thin
electrochemical cell in isothermal (constant temperature) and isobaric (constant pressure)
conditions, the heat generation rate | , (if heat of mixing is neglected27,28) is given by
340 341 | , = − + + ∆ Equation  342 343
where | , is positive if heat is released by the cell, is the current (positive for charging),
is the cell voltage, is the equilibrium potential, is the temperature, is the surrounding
pressure, and ∆ is the enthalpy of reaction of a chemical reaction (other than the main
electrochemical reaction) occurring at a rate . Recognizing the first term as irreversible heat
generation due to overpotential, the second term as reversible entropic heat, and the last term as
parasitic heat due to side reactions, Equation Error! Reference source not found. can also be
349 equivalently formulated as26 350 351 | , = + − ̃ + Equation  352 353
where is the cell’s overpotential (the product is always positive), is the number of
electrons involved in electrode reaction, is the Faraday’s constant, is the stoichiometric content
of Li in the positive electrode material, is the total entropy of the positive electrode material at a
given , ̃ is the molar entropy of Li metal negative electrode, and is the parasitic heat flow due
- 21 -
to other chemical reactions. These formulations have extensively been used for investigating the
entropic heat of intercalation materials45 and more recently the parasitic heat in Li-ion cells30,46–49.
For quantifying the entropy change, one possibility (potentiometric method) is to perform
temperature-dependent equilibrium potential measurements for directly determining in Equation
Error! Reference source not found..28,50–53 Another option (calorimetric method) is to measure ,
, and | , over a charge–discharge cycle and obtain the terms in Equation  while considering
these terms to be path independent (same on charge vs. discharge), which is a reasonable
assumption for classical intercalation materials only.26,30,49 Lastly, a method called electrothermal
impedance spectroscopy (ETIS) has also recently been developed.54 To understand the effect of
quasi-static voltage hysteresis, the irreversible heat term can be empirically modelled, when is
367 relatively low, as49 368 369 = + | | Equation  370 371
where is the cell’s internal resistance and the inherent quasi-static (extrapolated to
zero-current) voltage hysteresis. This equation was successfully applied to empirically model the
heat flow in LiNi0.4Mn0.4Co0.2O2/graphite cells by including a small (± ~4 mV) voltage hysteresis 374
equally on charge and discharge and by considering as a function of SoC only.49 However for
the Li-rich electrodes, this approach is not suitable because (i) they show a much larger hysteresis
(both Li-rich NMC and LRSO that are of interest in this work) and (ii) their is known to vary
differently on charge vs. discharge with SoC.5,9 Likewise, can be expected to differ as a
function of cell potential on charge vs. discharge in these highly path-dependent materials. In other
words, the position of in hysteretic Li-rich electrodes cannot simply be assumed in the middle of
the charge and discharge profiles, unlike in classical intercalation materials. We therefore use a
- 22 -
different approach herein that is based on “enthalpy potential”, as described in the main text.
Material synthesis and electrode fabrication. Single-phase Li2Ru0.75Sn0.25O3 (LRSO) 384
samples, as determined by X-ray powder diffraction, were obtained by solid-state synthesis reported
elsewhere.25 The Bellcore plastic method55 was used to prepare high-porosity self-standing 386
electrodes, as described in detail previously.9 The final electrode film was composed of 73% (by 387
weight) active material, 9% carbon SP (MM, Belgium), and 18% binder – poly(vinylidene
co-hexafluoropropylene) (PVDF-HFP) (Arkema). The film was designed for an active material
loading of ~20 mg cm–2, ~200 µm film-thickness, and ~60% porosity. Such a relatively high
loading was needed to generate reliable amounts of heat flow from the coin cells. Owing to the high
porosity of carefully designed electrodes, in addition to the relatively low C-rates studied herein, the
liquid-phase transport limitations (and their associated entropy production56,57) are expected to
remain very low compared to those in the solid phase, as also suggested via previous modelling57,58
Coin-cell assembly. Using ~1 cm2circular discs of this electrode film, 2032 coin-type cells
with Li metal foil as the negative electrode were assembled in an argon-filled glove-box with two
layers of 12 μm polyethylene film coated with 4μm alumina (W-SCOPE separators) along with one
layer of a WhatmanTM GF/D borosilicate glass microfiber sheet (GE Healthcare Life Sciences). The
electrolyte used was LP100 (Merck) having 1M LiPF6 in ethylene carbonate : propylene carbonate : 401
dimethyl carbonate in a 1 : 1 : 3 volume ratio. No stress build-up (mechanical work) is expected to
occur inside the cell owing to LRSO’s very small lattice volume change (maximum 3.7 %)25, along
with the use of a soft and deformable glass microfiber separator that can accommodate any residual
strain. The C-rate in this work is defined such that 1C corresponds to the removal of 1 Li per
formula unit of LRSO in one hour (1C = 160.13 mA g–1). 406
- 23 -
Isothermal Calorimetry. Depending on the experiment, the cells were pre-cycled at room
temperature before being transferred into a TAM III Microcalorimeter (TA Instruments: stability ±
0.0001 °C, accuracy ± 1 μW, precision ± 10 nW) for isothermal calorimetry measurements at 40 °C.
A few formation cycles were again carried out once the cells were inside the calorimeter. Such
cycling allows any possible side-reactions, such as gassing and/or surface stabilization in initial
cycles, to reach to a nearly steady state. The baseline drift over the course of the experiments did
not exceed ± 0.5 μW. The time constant of the calorimeter is about 5 minutes. All specifications
and information regarding microcalorimetry calibration, cell connections, and operation procedures
can be found in previous literature.30,46–49 The electrochemical cycling was performed with a
Maccor 4000 series cycler connected to the cells inside the calorimeter. Depending on the
experiment, either a constant current (CC) or a constant current constant voltage (CCCV) protocol
was used. The voltage hold of the CCCV step was terminated when current decayed to a low value
of C/100. The observed heat flow, defined positive when heat is generated by the cell, mainly arises
from the positive electrode. A constant and small value of background heat of +3.4 μW, accounting
for parasitic reactions, was subtracted from the raw measured heat flow values, irrespective of
cationic or anionic redox regime. Such an assumption of constant parasitic heat is acceptable given
the scope of this study. Still, it must be kept in mind that parasitic heat depends on the complex
relationship among the cathode, the anode, the electrolyte, the operating conditions (cell voltage
etc.), the cell history over the course of the experiment, besides the continuous corrosion of inactive
- 24 -
The authors declare that the main data supporting the findings of this study are available
within the article and its Supporting Information files. Extra data are available from the
corresponding author upon reasonable request.
* Corresponding authors:
C. Delacourt: firstname.lastname@example.org
J.-M. Tarascon: email@example.com
J.M.T. and G.A. acknowledge the funding from the European Research Council (ERC)
(FP/2014)/ERC Grant-Project 670116-ARPEMA. S.L.G thanks NSERC and the Walter C. Sumner
Foundation for funding. We are grateful to Dr. Jeff Dahn for providing access to some of the
equipment used in this work.
G.A. and S.L.G. conceived the idea. G.A. prepared the electrochemical cells and S.L.G.
performed the isothermal calorimetry experiments. G.A. and C.D. performed the thermodynamic
analysis. J.M.T. supervised the project. G.A. wrote the paper, with contributions from all authors.
Competing Financial Interests
The authors declare no competing financial interests.
- 25 -
1. Zheng, J. et al. Li- and Mn-Rich Cathode Materials: Challenges to Commercialization. Adv. Energy Mater. 1601284 (2016). doi:10.1002/aenm.201601284
2. Manthiram, A., Knight, J. C., Myung, S.-T., Oh, S.-M. & Sun, Y.-K. Nickel-Rich and Lithium-Rich Layered Oxide Cathodes: Progress and Perspectives. Adv. Energy Mater. 6, 1501010 (2016).
3. Myung, S.-T. et al. Nickel-rich Layered Cathode Materials for Automotive Lithium-ion
Batteries: Achievements and Perspectives. ACS Energy Lett. (2016). doi:10.1021/acsenergylett.6b00594
4. Luo, K. et al. Charge-compensation in 3d-transition-metal-oxide intercalation cathodes through
the generation of localized electron holes on oxygen. Nat. Chem. 8, 684–691 (2016).
5. Assat, G. et al. Fundamental interplay between anionic/cationic redox governing the kinetics
and thermodynamics of lithium-rich cathodes. Nat. Commun. 8, Article number: 2219 (2017). 6. Gent, W. E. et al. Coupling between oxygen redox and cation migration explains unusual
electrochemistry in lithium-rich layered oxides. Nat. Commun. 8, (2017).
7. Assat, G. & Tarascon, J.-M. Fundamental understanding and practical challenges of anionic redox activity in Li-ion batteries. Nat. Energy 1 (2018). doi:10.1038/s41560-018-0097-0 8. Croy, J. R. et al. Examining Hysteresis in Composite x Li2MnO3 · (1–x) LiMO2 Cathode
Structures. J. Phys. Chem. C 117, 6525–6536 (2013).
9. Assat, G., Delacourt, C., Corte, D. A. D. & Tarascon, J.-M. Editors’ Choice—Practical
Assessment of Anionic Redox in Li-Rich Layered Oxide Cathodes: A Mixed Blessing for High Energy Li-Ion Batteries. J. Electrochem. Soc. 163, A2965–A2976 (2016).
10. Dees, D. W. et al. Electrochemical Modeling and Performance of a Lithium- and Manganese-Rich Layered Transition-Metal Oxide Positive Electrode. J. Electrochem. Soc. 162, A559– A572 (2015).
11. Croy, J. R., Balasubramanian, M., Gallagher, K. G. & Burrell, A. K. Review of the U.S. Department of Energy’s ‘Deep Dive’ Effort to Understand Voltage Fade in Li- and Mn-Rich Cathodes. Acc. Chem. Res. 48, 2813–2821 (2015).
12. Meister, P. et al. Best Practice: Performance and Cost Evaluation of Lithium Ion Battery Active Materials with Special Emphasis on Energy Efficiency. Chem. Mater. 28, 7203–7217 (2016). 13. Ohzuku, T., Nagayama, M., Tsuji, K. & Ariyoshi, K. High-capacity lithium insertion materials
of lithium nickel manganese oxides for advanced lithium-ion batteries: toward rechargeable capacity more than 300 mA h g−1. J. Mater. Chem. 21, 10179 (2011).
- 26 -
14. Maitra, U. et al. Oxygen redox chemistry without excess alkali-metal ions in Na2/3[Mg0.28Mn0.72]O2. Nat. Chem. (2018). doi:10.1038/nchem.2923
15. Mortemard de Boisse, B. et al. Intermediate honeycomb ordering to trigger oxygen redox chemistry in layered battery electrode. Nat. Commun. 7, 11397 (2016).
16. Yabuuchi, N. et al. Origin of stabilization and destabilization in solid-state redox reaction of oxide ions for lithium-ion batteries. Nat. Commun. 7, 13814 (2016).
17. A. House, R. et al. Lithium manganese oxyfluoride as a new cathode material exhibiting oxygen redox. Energy Environ. Sci. (2018). doi:10.1039/C7EE03195E
18. Croy, J. R., Gallagher, K. G., Balasubramanian, M., Long, B. R. & Thackeray, M. M.
Quantifying Hysteresis and Voltage Fade in x Li2MnO3 ● (1-x) LiMn0.5Ni0.5O2 Electrodes as a
Function of Li2MnO3 Content. J. Electrochem. Soc. 161, A318–A325 (2014).
19. Konishi, H. et al. Electrochemical reaction mechanisms under various charge-discharge operating conditions for Li1.2Ni0.13Mn0.54Co0.13O2 in a lithium-ion battery. J. Solid State Chem.
262, 294–300 (2018).
20. Dogan, F. et al. Re-entrant Lithium Local Environments and Defect Driven Electrochemistry of Li- and Mn-Rich Li-Ion Battery Cathodes. J. Am. Chem. Soc. 137, 2328–2335 (2015).
21. Kleiner, K. et al. Origin of High Capacity and Poor Cycling Stability of Li-Rich Layered Oxides: A Long-Duration in Situ Synchrotron Powder Diffraction Study. Chem. Mater. 30, 3656–3667 (2018).
22. Konishi, H. et al. Origin of hysteresis between charge and discharge processes in lithium-rich layer-structured cathode material for lithium-ion battery. J. Power Sources 298, 144–149 (2015).
23. Assat, G., Iadecola, A., Delacourt, C., Dedryvère, R. & Tarascon, J.-M. Decoupling Cationic– Anionic Redox Processes in a Model Li-rich Cathode via Operando X-ray Absorption
Spectroscopy. Chem. Mater. (2017). doi:10.1021/acs.chemmater.7b03434
24. Rinaldo, S. G. et al. Physical Theory of Voltage Fade in Lithium- and Manganese-Rich Transition Metal Oxides. J. Electrochem. Soc. 162, A897–A904 (2015).
25. Sathiya, M. et al. Reversible anionic redox chemistry in high-capacity layered-oxide electrodes.
Nat. Mater. 12, 827–835 (2013).
26. Dahn, J. R. et al. Entropy of the intercalation compound LixMo6Se8 from calorimetry of
electrochemical cells. Phys. Rev. B 32, 3316–3318 (1985).
27. Thomas, K. E. & Newman, J. Thermal Modeling of Porous Insertion Electrodes. J.
Electrochem. Soc. 150, A176 (2003).
- 27 -
Power Sources 119–121, 844–849 (2003).
29. Kondepudi, D. & Prigogine, I. Modern thermodynamics: from heat engines to dissipative
structures. (Wiley & Sons, 2015).
30. Glazier, S. L., Nelson, K. J., Allen, J. P., Li, J. & Dahn, J. R. The Effect of Different Li(Ni 1-x-yMnxCoy)O2 Positive Electrode Materials and Coatings on Parasitic Heat Flow as Measured by
Isothermal Microcalorimetry, Ultra-High Precision Coulometry and Long Term Cycling. J.
Electrochem. Soc. 164, A1203–A1212 (2017).
31. Shi, W. et al. The Effect of Entropy and Enthalpy Changes on the Thermal Behavior of Li-Mn-Rich Layered Composite Cathode Materials. J. Electrochem. Soc. 163, A571–A577 (2016). 32. Salager, E. et al. Solid-State NMR of the Family of Positive Electrode Materials Li2Ru1–ySnyO3
for Lithium-Ion Batteries. Chem. Mater. 26, 7009–7019 (2014).
33. Bard, A. J. & Faulkner, L. R. Electrochemical methods: fundamentals and applications. (Wiley, 2001).
34. Sauvage, J.-P. Transition Metal-Containing Rotaxanes and Catenanes in Motion: Toward Molecular Machines and Motors. Acc. Chem. Res. 31, 611–619 (1998).
35. Sano, M. & Taube, H. ‘Molecular hysteresis’ in an electrochemical system revisited. Inorg.
Chem. 33, 705–709 (1994).
36. Sano, M. Mechanism of the molecular hysteresis. Polym. Adv. Technol. 6, 178–184 (1995). 37. Rouxel, J. Anion–Cation Redox Competition and the Formation of New Compounds in Highly
Covalent Systems. Chem. – Eur. J. 2, 1053–1059 (1996).
38. Boisse, B. M. de et al. Highly Reversible Oxygen-Redox Chemistry at 4.1 V in Na4/7−x[□1/7Mn6/7]O2 (□: Mn Vacancy). Adv. Energy Mater. 0, 1800409
39. Zheng, T. & Dahn, J. R. Hysteresis observed in quasi open-circuit voltage measurements of lithium insertion in hydrogen-containing carbons. J. Power Sources 68, 201–203 (1997). 40. Zheng, T., McKinnon, W. R. & Dahn, J. R. Hysteresis during Lithium Insertion in Hydrogen‐
Containing Carbons. J. Electrochem. Soc. 143, 2137–2145 (1996).
41. Yu, H.-C. et al. Designing the next generation high capacity battery electrodes. Energy Environ.
Sci. 7, 1760 (2014).
42. Inaba, M., Fujikawa, M., Abe, T. & Ogumi, Z. Calorimetric Study on the Hysteresis in the Charge-Discharge Profiles of Mesocarbon Microbeads Heat-Treated at Low Temperatures. J.
Electrochem. Soc. 147, 4008–4012 (2000).
43. Bernardi, D., Pawlikowski, E. & Newman, J. A general energy balance for battery systems. J.
Electrochem. Soc. 132, 5–12 (1985).
- 28 - systems. J. Electrochem. Soc. 144, 2697–2704 (1997).
45. Bandhauer, T. M., Garimella, S. & Fuller, T. F. A Critical Review of Thermal Issues in Lithium-Ion Batteries. J. Electrochem. Soc. 158, R1 (2011).
46. Krause, L. J., Jensen, L. D. & Dahn, J. R. Measurement of Parasitic Reactions in Li Ion Cells by Electrochemical Calorimetry. J. Electrochem. Soc. 159, A937–A943 (2012).
47. Downie, L. E. & Dahn, J. R. Determination of the Voltage Dependence of Parasitic Heat Flow in Lithium Ion Cells Using Isothermal Microcalorimetry. J. Electrochem. Soc. 161, A1782– A1787 (2014).
48. Downie, L. E., Hyatt, S. R., Wright, A. T. B. & Dahn, J. R. Determination of the Time Dependent Parasitic Heat Flow in Lithium Ion Cells Using Isothermal Microcalorimetry. J.
Phys. Chem. C 118, 29533–29541 (2014).
49. Downie, L. E., Hyatt, S. R. & Dahn, J. R. The Impact of Electrolyte Composition on Parasitic Reactions in Lithium Ion Cells Charged to 4.7 V Determined Using Isothermal
Microcalorimetry. J. Electrochem. Soc. 163, A35–A42 (2016).
50. Wen, C. J. & Huggins, R. A. Thermodynamic Study of the Lithium‐Tin System. J.
Electrochem. Soc. 128, 1181–1187 (1981).
51. Dahn, J. R. & Haering, R. R. Entropy measurements on LixTiS2. Can. J. Phys. 61, 1093–1098
52. Reynier, Y., Yazami, R. & Fultz, B. The entropy and enthalpy of lithium intercalation into graphite. J. Power Sources 119–121, 850–855 (2003).
53. Forgez, C., Vinh Do, D., Friedrich, G., Morcrette, M. & Delacourt, C. Thermal modeling of a cylindrical LiFePO4/graphite lithium-ion battery. J. Power Sources 195, 2961–2968 (2010).
54. Schmidt, J. P., Weber, A. & Ivers-Tiffée, E. A novel and precise measuring method for the entropy of lithium-ion cells: ΔS via electrothermal impedance spectroscopy. Electrochimica
Acta 137, 311–319 (2014).
55. Tarascon, J.-M., Gozdz, A. S., Schmutz, C., Shokoohi, F. & Warren, P. C. Performance of Bellcore’s plastic rechargeable Li-ion batteries. Solid State Ion. 86, 49–54 (1996).
56. Kjelstrup, S. & Bedeaux, D. Non-equilibrium Thermodynamics of Heterogeneous Systems. (World Scientific, 2008).
57. Richter, F., Gunnarshaug, A., Burheim, O. S., Vie, P. J. S. & Kjelstrup, S. Single Electrode Entropy Change for LiCoO 2 Electrodes. ECS Trans. 80, 219–238 (2017).
58. Santhanagopalan, S., Guo, Q., Ramadass, P. & White, R. E. Review of models for predicting the cycling performance of lithium ion batteries. J. Power Sources 156, 620–628 (2006). 59. Malifarge, S., Delobel, B. & Delacourt, C. Experimental and Modeling Analysis of Graphite
- 29 -
Electrodes with Various Thicknesses and Porosities for High-Energy-Density Li-Ion Batteries.
1.2 0.9 0.6 0.3 0.0 2 3 4 5 2.0 1.5 1.0 0.5 0.0 2 3 4 5 0 80 160 240 2 3 4 5 0 80 160 240 2 3 4 5 a Cell Volta ge (V) x in LixNi0.13Mn0.54Co0.13O2 A C A C A C A C Li-rich NMC 'practical' electrode
first cycle first cycle
b LRSO 'model' electrode Cell Volta ge (V) x in LixRu0.75Sn0.25O3 A C A C next cycles d 91 % energy efficiency Volta ge (V) Capacity (mAh g–1) next cycles c Volta ge (V) Capacity (mAh g–1) 87 % energy efficiency
0 40 80 120 3.0 3.4 3.8 3.0 3.4 3.8 0 40 80 120 0 1 2 3.0 3.4 3.8 0 40 80 120 3.0 3.4 3.8 0 8 16 24 32 40 0 10 20 30 Cell Volta ge (V) Capacity (mAh g–1) C/5 C/7.14 C/10 C/20 a b charge - solid discharge - dashed Cell Volta ge an d Ent ha lpy Po ten tial (V) UH V C/20 Rate of Heat Flow (mW g –1) Capacity (mAh g–1) c Ent ha lpy Po ten tial (V) C/5 C/7.14 C/10 C/20 charge discharge Capacity (mAh g–1) d C/5 C/7.14 C/10
Lost Electrical Work
Waste Heat Net He at an d Work (W h kg –1) Current (mA g–1) C/20
1.8 2.4 3.0 3.6 4.2 4.8 0 60 120 180 240 300 0 60 120 180 240 300 0 8 16 24 32 0 60 120 180 240 300 1.8 2.4 3.0 3.6 4.2 4.8 a C/5 Cell Volta ge (V) charge (solid) discharge (dashed) * * b * cycler interrupt Rate of Heat Flow (mW g –1 ) Capacity (mAh g–1) C/5 c V charge (solid) discharge (dashed) Capacity (mAh g–1) * Cell Volta ge an d Ent ha lpy Po ten tial (V) UH V
0 80 160 240 2.2 3.0 3.8 4.6 2.2 3.0 3.8 4.6 0 80 160 240 0.0 0.5 1.0 2.2 3.0 3.8 4.6 0 80 160 240 2.2 3.0 3.8 4.6 0 8 16 24 32 40 0 50 100 150 Cell Volta ge (V) Capacity (mAh g–1) C/5 C/10 C/25 C/50 a C/50 b charge (solid) discharge (dashed) Cell Volta ge an d Ent ha lpy Po ten tial (V) UH V Rate of Heat Flow (mW g –1) Capacity (mAh g–1) c Ent ha lpy Po ten tial (V) C/5 C/10 C/25 C/50 charge discharge Capacity (mAh g–1) d C/5 C/25 C/10
Lost Electrical Work
Waste Heat Net He at an d Work (W h kg –1) Current (mA g–1) C/50 b
2.2 3.0 3.8 4.6 0 20 40 60 80 100 0 80 160 240 0 4 8 12 0 80 160 240 2.2 3.0 3.8 4.6 0 20 40 60 80 100 0 60 120 0 20 40 60 80 100 SoC (%) Cell Volta ge (V)
charge window opening
a b Rate of Heat Flow (mW g –1 ) Capacity (mAh g–1) discharge only c Cell Volta ge an d Ent ha lpy Po ten tial (V) Capacity (mAh g–1)
UH for discharge only
Lost Electrical Work
Waste Heat Net Hea t a nd Work (W h kg –1 ) SoC (%) SoC (%)
A Ar+ A+ Ar C C+ non-eq. dis non-eq. ch redox A A+ Ar+ Ar Gibb s f ree en erg y discharged charged EC EC C C c Anionic Redox b a Cationic Redox